Both minor and major repairs as well as extensive remodeling are common in existing swimming pool structures. Removal and replacement of portions of a pool structure is perfectly acceptable as long as the procedures listed below are followed for attaining proper bonding of the new repair materials to the existing swimming pool structure.
It is not uncommon to encounter hollowness or other surface defects in pneumatically applied concrete or mortar in swimming pool construction. Hollowness, when tapped with a metal object, is an indication that the surface of the pneumatically applied material is not bonded to the underlining substrate. It is likely that “rebound” was placed or allowed to remain on the surface in these localized areas and has de-laminated from the underlining substrate.
Rebound is typically made up of the larger and harder particles (which tend to ricochet) and does not contain adequate cement, water or density to develop significant strength. Rebound, therefore, should not be used in any application where strength, hardness or durability is needed. Rebound is frequently encountered on horizontal surfaces such as the pool floor, shallow end access steps and the tops of the below water benches.
Rebound on or near the gunite surface is or may become delaminated in the future and should be removed prior to the pool’s plaster surface application. The removal can best be accomplished by the use of light weight, pneumatic jack hammers which will remove the soft or delaminated rebound without damaging the structural shell.
The following procedures must be followed for attaining proper bonding of the new repair materials to the existing swimming pool structure.
1. Existing surfaces must be sound, free of defects, clean and free of bond inhibiting materials.
2. Existing surfaces must be roughened by chipping or other suitable means to provide an open pore structure. All loose, cracked or deteriorated materials must be removed.
3. Clean existing surfaces by water blasting.
5. Saturated surface dry condition of the substrate shall be maintained to prevent premature drying of the bonding paste.
6. Any reinforcement exposed in the repair or remodeling must be completely exposed with a minimum of 1 inch clear completely around the reinforcement to permit proper encasement of the reinforcement in the repair material.
7. Where it is impractical to use pneumatically applied material for the repair, dry pack mortar (low water content) may be used for small repairs to minimize the potential for shrinkage cracking. Pre-packaged products such as Rapid-Set Mortar Mix (for thinner repairs) or Rapid-Set Concrete Mix (for thicker repairs) are low shrinkage, fast setting products formulated for repair applications and are ideal for minor repairs in swimming pool. When using pre-packaged products, it is critical that the manufacturers use limitations, mixing and placing instructions be explicitly followed.
8. When using Dry Pack Mortar or equivalent, the material should be applied over cement paste or another approved bonding agent, which has been brushed onto the substrate (existing material) for absorption into the pore structure. The new material shall be applied before the cement paste or other approved bonding agent “skins over” or starts its “setting stage”. Bonding aids are generally not required when pneumatically applied materials are utilized in the repair.
Copyright © 2012 Pool Engineering, Inc.
Click Here to go Back to List of General Policies